Biomaterials in oral and maxillofacial surgery/rotary endodontic courses by indian dental academy
Biomaterials In oral and maxillofacial surgery
Biomaterial is used to make devices to replace a part or a function of the body in
a safe, reliable, economic, and physiologically acceptable manner.
A variety of devices and materials presently used in the treatment of disease or
injury include such common place items as sutures, needles, catheters, plates,
tooth fillings, etc.
The use of biomaterials did not become practical until the advent of an aseptic
surgical technique developed by Dr. J. Lister in the 1860s. Earlier surgical
procedures, whether they involved biomaterials or not, were generally
unsuccessful as a result of infection. Problems of infection tend to be
exacerbated in the presence of biomaterials, since the implant can provide a
region inaccessible to the body’s immunologically competent cells. The earliest
successful implants, as well as a large fraction of modern ones, were in the
Definitions of biomaterials :
1) A Biomaterial can be simply defined as a synthetic material used to
replace part of a living system or to function in intimate contact with living
2) The Clemson University Advisory Board for Biomaterials has formally
defined a biomaterial to be “a systemically and pharmacologically inert
substance designed for implantation within or incorporation with living
3) Black (1992) defined biomaterials as “a nonviable material used in a
medical device, intended to interact with biological systems”.
4) Bruck (1980) defined biomaterials as “materials of synthetic as well as of
natural origin in contact with tissue, blood, and biological fluids, and
intended for use for prosthetic, diagnostic, therapeutic, and storage
applications without adversely affecting the living organism and its
5) Williams (1987) defined the biomaterials as “any substance (other than
drugs) or combination of substances, synthetic or natural in origin, which
can be used for any period of time, as a whole or as a part of a system
which treats, augments, or replaces any tissue, organ, or function of the
Types of biomaterials :
I) Metallic biomaterials
Metals are used as biomaterials due to their excellent electrical and thermal
conductivity and mechanical properties. Since some electrons are independent in
metals, they can quickly transfer an electric charge and thermal energy. The
mobile free electrons act as the binding force to hold the positive metal ions
together. This attraction is strong, as evidenced by the closely packed atomic
arrangement resulting in high specific gravity and high melting points of most
metals. Since the metallic bond is essentially nondirectional, the position of the
metal ions can be altered without destroying the crystal structure resulting in a
plastically deformable solid.
The first metal alloy developed specifically for human use was the “vanadium
steel” which was used to manufacture bone fracture plates (Sherman plates) and
screws. Most metals such as iron (Fe), chromium (Cr), cobalt (Co), nickel (Ni),
titanium (Ti), tantalum (Ta), niobium (Nb), molybdenum (Mo), and tungsten (W)
that were used to make alloys for manufacturing implants can only be tolerated
by the body in minute amounts. Sometimes those metallic elements, in naturally
occurring forms, are essential in red blood cell functions (Fe) or synthesis of a
vitamin B 12 (Co), but cannot be tolerated in large amounts in the body [Black,
1) Stainless Steel
2) CoCr Alloys
3) Ti Alloys
A) Pure Ti and Ti6Al4V
B) TiNi Alloys
4) Dental Metals
5) Other Metals
1) Stainless steel :
The first stainless steel utilized for implant fabrication was the 18-8 (type 302 in
modern classification), which is stronger and more resistant to corrosion than the
Later 18-8s Mo stainless steel was introduced which contains a small percentage
of molybdenum to improve the corrosion resistance in chloride solution (salt
water). This alloy became known as type 316 stainless steel.
In the 1950s the carbon content of 316 stainless steel was reduced from 0.08 to a
maximum amount of 0.03% (all are weight percent unless specified) for better
corrosion resistance to chloride solution and to minimize the sensitization, and
hence became known as type 316L stainless steel.
The minimum effective concentration of chromium is 11% to impart corrosion
resistance in stainless steels. The chromium is a reactive element, but it and its
alloys can be passivated by 30% nitric acid to give excellent corrosion resistance.
The austenitic stainless steels, especially types 316 and 316L , are most widely
used for implant fabrication. These cannot be hardened by heat treatment but
can be hardened by cold-working. This group of stainless steels is nonmagnetic
and possesses better corrosion resistance than any others. The inclusion of
molybdenum enhances resistance to pitting corrosion in salt water.
Compositions of 316L Stainless Steel
(American Society for Testing and Materials)
Element Composition (%)
Carbon 0.03 max
Manganese 2.00 max
Phosphorus 0.03 max
Sulfur 0.03 max
Silicon 0.75 max
2) Cobalt chromium ( Co Cr) alloys :
There are basically two types of cobalt-chromium alloys:
1) The castable CoCrMo alloy
2) The CoNiCrMo alloy which is usually Wrought by (hot) forging .
The castable CoCrMo alloy has been used for many decades in dentistry and,
relatively recently, in making artificial joints.
The wrought CoNiCrMo alloy is relatively new, now used for making the stems of
prosthesis for heavily loaded joints such as the knee and hip.
The ASTM lists four types of CoCr alloys which are recommended for surgical
1) cast CoCrMo alloy (F75)
2) wrought CoCrWNi alloy (F90)
3) wrought CoNiCrMo alloy (F562),
4) wrought CoNiCrMoWFe alloy (F563).
At the present time only two of the four alloys are used extensively in implant
fabrications, the castable CoCrMo and the wrought CoNiCrMo alloy.
The two basic elements of the CoCr alloys form a solid solution of up to 65% Co.
The molybdenum is added to produce finer grains which results in higher
strengths after casting or forging. The chromium enhances corrosion resistance
as well as solid solution strengthening of the alloy.
The CoNiCrMo alloy originally called MP35N (Standard Pressed Steel Co.) contains
approximately 35% Co and Ni each. The alloy is highly corrosion resistant to
seawater (containing chloride ions) under stress. However, there is a
considerable difficulty of cold working on this alloy, especially when making large
devices such as hip joint stems. Only hot-forging can be used to fabricate a large
implant with the alloy.
3) Titanium Alloys :
A) Pure Titanium and Ti6Al4V :
Titanium used for implant fabrication since 1930s.
Titanium’s lightness (4.5 g/cm3
) and good mechanochemical properties
are salient features for implant application.
There are four grades of unalloyed commercially pure (cp) titanium for surgical
The impurity contents separate them; oxygen, iron, and nitrogen should be
controlled carefully. Oxygen in particular has a great influence on the ductility
The main alloying elements of the alloy are aluminum (5.5~6.5%) and vanadium
Titanium is an allotropic material, which exists as a hexagonal close packed
structure up to 882°C and body-centered cubic structure above that
temperature. Titanium alloys can be strengthened and mechanical properties
varied by controlled composition and thermomechanical processing techniques.
The addition of alloying elements to titanium enables it to have a wide range of
(1) Aluminum tends to stabilize the alpha-phase, that is increase the
transformation temperature from alpha to beta -phase
(2) vanadium stabilizes the beta-phase by lowering the temperature of the
transformation from alpha to beta phase.
The alpha-alloy has a single-phase microstructure which promotes good
weldability. The stabilizing effect of the high aluminum content of these groups
of alloys makes excellent strength characteristics and oxidation resistance at high
temperature (300~600°C). These alloys cannot be heat treated for precipitation
hardening since they are single-phased.
The addition of controlled amounts of beta-stabilizers causes the higher strength
beta-phase to persist below the transformation temperature which results in the
two-phase system. The precipitates of beta-phase will appear by heat treatment
in the solid solution temperature and subsequent quenching, followed by aging
at a somewhat lower temperature.
The aging cycle causes the coherent precipitation of some fine alpha particles
from the metastable beta particles;
Imparting alpha structure may produce local strain field capable of absorbing
deformation energy. Cracks are stopped or deterred at the alpha particles, so
that the hardness is higher than for the solid solution.
The higher percentage of beta-stabilizing elements (13%V in Ti13V11Cr3Al alloy)
results in a microstructure that is substantially beta which can be strengthened
by heat treatment. Another Ti alloy (Ti13Nb13Zr) with 13% Nb and 13% Zr
showed martensite structure after being water quenched and aged, which
showed high corrosion resistance with low modulus (E = 79 MPa).
Formation of plates of martensite induces considerable elastic distortion in the
parent crystal structure and increases strength.
B) TiNi Alloys
The titanium–nickel alloys show unusual properties i.e., after it is deformed the
material can snap back to its previous shape following heating of the material. This
phenomenon is called shape memory effect (SME). The SME of TiNi alloy was
first observed by Buehler and Wiley at the U.S. Naval Ordnance Laboratory
[Buehler et al., 1963].
The equiatomic TiNi or NiTi alloy (Nitinol) exhibits an exceptional SME near
room temperature: if it is plastically deformed below the transformation
temperature, it reverts back to its original shape as the temperature is raised. The
SME can be generally related to a diffusionless martensitic phase transformation
which is also thermoelastic in nature, the thermoelasticity being attributed to the
ordering in the parent and martensitic phases [Wayman and Shimizu, 1972].
Another unusual property is the superelasticity. As can be seen, the stress does
not increase with increased strain after the initial elastic stress region and upon
release of the stress or strain the metal springs back to its original shape in
contrast to other metals such as stainless steel. The superlastic property is
utilized in orthodontic archwires since the conventional stainless steel wires are
too stiff and harsh for the tooth. In addition, the shape memory effect can also be
Some possible applications of shape memory alloys are orthodontic dental
archwire, intracranial aneurysm clip, vena cava filters , contractile artificial
muscles for an artificial heart, vascular stent, catheter guide wire, and orthopedic
staple [Duerig et al., 1990]
4) Dental metals :
A. Dental amalgam
B. Gold and gold alloys
5) Other metals :
B. Platinum group metals (PGM) such as Pt, Pd, Rh, Ir, Ru, and Os
II) CERAMIC BIOMATERIALS
1) Nonabsorbable or Relatively Bioinert Bioceramics
A. Pyrolitic carbon-coated devices
B. Dense and nonporous aluminum oxides
C. Porous aluminum oxides
D. Zirconia ceramics
E. Dense hydroxyapatites
2) Biodegradable or Resorbable Ceramics
A. Aluminum–calcium–phosphorous oxides
B. Glass fibers and their composites
D. Calcium sulfates, including plaster of Paris
E. Ferric–calcium–phosphorous oxides
G. Tricalcium phosphate
H. Zinc–calcium–phosphorous oxides
I. Zinc–sulfate–calcium–phosphorous oxides
3) Bioactive or Surface-Reactive Ceramics
A. Bioglass and Ceravital
B. Dense and nonporous glasses
III) Polymeric Biomaterials
1) Polyvinylchloride (PVC)
2) Polyethylene (PE)
3) Polypropylene (PP)
4) Polymethylmetacrylate (PMMA)
5) Polystyrene (PS)
6) Polyethylenterephthalate (PET)
7) Polytetrafluoroethylene (PTFE)
8) Polyurethane (PU)
9) Polyamide (nylon)
IV) Composite biomaterials
Some applications of composites in biomaterial applications are:
(1) dental filling composites
(2) reinforced methyl methacrylate bone cement and ultra-high-molecular-
(3) orthopedic implants with porous surfaces.
V) Biodegradable Polymeric Biomaterials
1) Glycolide/Lactide-Based Biodegradable Linear Aliphatic polyesters
A. Glycolide-Based Biodegradable Homopolymer Polyesters
B. Glycolide-Based Biodegradable Copolyesters Having Aliphatic
C. Glycolide-Based Biodegradable Copolyesters with Non-Aliphatic Polyester-
D. Glycolide-Derived Biodegradable Polymers Having Ether Linkage
E. Lactide Biodegradable Homopolymers and Copolymers
2) Non-Glycolide/Lactide-Based Linear Aliphatic Polyesters
3) Non-Aliphatic Polyesters Type Biodegradable Polymers
A. Aliphatic and Aromatic Polycarbonates
B. Poly(alkylene oxalates) and Copolymers